Dendritic Polyglycerol Sulfate Hydrogels as a Potential Viscosupplement for Treatment of
to obtain the academic degree Doctor rerum naturalium (Dr. rer. nat.)
submitted to the Department of Biology, Chemistry and Pharmacy.
Shabnam Hemmati-Sadeghi from Iran
Declaration of honesty
Hereby I declare and confirm that this PhD thesis is entirely the result of my own work and that no other sources than those cited have been used. All annotations, which have been used from published or unpublished sources, are identified as such. The shown illustrations have been created by myself or have been marked with the corresponding references.
Shabnam Hemmati-Sadeghi April 2018
This PhD thesis was carried out within the research groups of Prof. Dr. Rainer Haag and Prof.
Dr. Michael Sittinger from April 2015 to April 2018 at the Institute of Chemistry and Biochemistry of the Freie Universität Berlin, Tissue Engineering Laboratory of Charité - Universitätsmedizin Berlin, and Berlin-Brandenburg School for Regenerative Therapies (BSRT). This study has been funded by Dahlem Research School (DRS) and Berlin- Brandenburg School for Regenerative Therapies (BSRT) with grant number GSC203.
1. Reviewer: Prof. Dr. Rainer Haag, Freie Universität Berlin
2. Reviewer: Prof. Dr. Michael Sittinger, Charité – Universitätsmedizin Berlin
Day of defense:08.06.2018
Completion of this doctoral dissertation was only possible with the support of several people and I would like to express my sincere gratitude to all of them. First of all, I would like to express my gratitude to Prof. Dr. Rainer Haag and Prof. Dr. Michael Sittinger for giving me the opportunity to work in their dynamic groups, for the valuable discussions, and especially for the constant positive response and motivation in all situations. I am also thankful for the excellent examples they have provided as successful leaders and professors.
I would like to thank Dr. Jochen Ringe for being my scientific mentor. I appreciate all his contribution of time and ideas as well as his effective suggestions that stopped me from spending too much time and effort on dead-end theories.
Furthermore, I sincerely thank Dr. Tilo Dehne for teaching me all the technical skills and his dedicated assistance through all kinds of problems. Thank you for your constant help, interest in my work, and your friendly support.
In addition, I would like to thank all former and present members of the Haag group and Sittinger group, Prof. Dr. Mohsen Adeli, Dr. Marion Haag, Dr. Stefan Stich, and particularly Dr. Kristin Fröhlich for their useful feedback regarding the progress of my work, Ingrid Semjonow, Anja Wachtel, Samuel Vetterlein, Dr. Pradip Dey, Suman Chowdhury, and Anja Stöshel for the daily support in lab work and material synthesis.
Further thanks go to my other lab colleagues, Nadia Sinner, Abbas Faghani, Benjamin von Lospichl, and my first student that I supervised, Johannes Weber, for the nice atmosphere and useful scientific as well as private discussions. I want to thank Dr. Pamela Winchester for proofreading my thesis and manuscripts. Sincere thanks go to Dr. Wiebke Fischer, Eike Ziegler, Heike Augst, Dr. Sabine Bartosch, and Bianca Kühn for helping me with financial regulations and complicated paper work as well as administrative issues. My heartfelt gratitude also goes to my special friend and colleague Leila Amini who helped me a lot during the last 3 years.
I am also grateful to Dr. Philipp Krüger, Dr. Michaela Endres, and all other employees of the company 'Trans Tissue Technologies'. The group has been a source of friendship as well as good advice and collaboration. At this point, I would like to thank Dr.
Sylvia Hondke for her critical and helpful comments.
Lastly, I would like to thank my family and friends for all their love and encouragement. To my parents, thank you for encouraging me in all of my pursuits and inspiring me to follow my dreams. I am especially grateful to my sister, Sharareh, who
supported me emotionally and financially. I always knew that you believed in me and wanted the best for me. I especially want to thank my husband for his love, care, and understanding throughout all these years. Merc eshgh.
List of abbreviations
3D 3 dimensional
ACR American College of Rheumatology
ADAMTS A disintegrin and metalloproteinase with thrombospondin motifs
BCP Basic calcium phosphate
CCL2 C-C motif chemokine 2
Col2A1 Collagen type II alpha 1 chain
COMP Cartilage oligomeric matrix compound CuAAC Copper-catalyzed alkyne–azide cycloaddition
dPG Dendritic polyglycerol
dPGS Dendritic polyglycerol sulfate
ECM Extra cellular matrix
EULAR European League Against Rheumatism
Fis1 Fission protein 1
HA Hyaluronic acid
LOX-1 Lectin-like oxidized LDL (low-density lipoprotein) receptor 1 MMPs Matrix metalloproteinases
NF-kB Nuclear factor kappa B
NSAIDs Non-steroidal anti-inflammatory drugs
OARSI Osteoarthritis Research Society International oxLDL Oxidized low-density lipoprotein
PEG-DIC Polyethylene glycol-dicyclooctyne
PRG4 Proteoglycan 4
RT-PCR Real-time polymer chain reaction SADOA Slow-acting drugs in osteoarthritis
SASP Senescence-associated secretory phenotype
SF Synovial fluid
siRNA Small interfering ribonucleic acid
SnCs Senescence cells
SOX9 SRY-homeobox-like 9
SPAAC Strain-promoted azide-alkyne cycloaddition STAT3 Signal transducer and activator of transcription 3
SZ Superficial zone
TNF-α Tumor necrosis factor-alpha
Table of contents
1 Introduction ... 1
1.1 Synovial joint... 1
1.1.1 Synovial membrane ... 2
1.1.2 Synovial fluid ... 2
1.1.3 Articular cartilage ... 2
1.2 Osteoarthritis ... 4
1.2.1 Main factors and players ... 6
1.2.2 Conventional treatments ... 8
1.2.3 Viscosupplementation with hyaluronic acid ... 9
1.3 Hydrogels ... 10
1.3.1 Injectable hydrogels for viscosupplementation in osteoarthritis ... 12
1.3.2 Polyethylene glycol and dendritic polyglycerol sulfate as building blocks for injectable in situ hydrogels ... 15
1.4 In vitro investigation of potential treatments for OA ... 17
1.4.1 Load-based in vitro models ... 18
1.4.2 Cytokine-based in vitro models ... 19
2 Scientific goal ... 21
3 Publication and Manuscripts ... 22
3.1 Hydrolytically degradable, dendritic polyglycerol sulfate based injectable hydrogels using strain promoted azide–alkyne cycloaddition reaction ... 22
3.2 Injectable hydrogels for treatment of osteoarthritis – A rheological study ... 32
3.3 TNF-induced biomimetic sulfated PEG-hydrogel inhibits proteoglycan loss and TNF- induced expression pattern in an osteoarthritis in vitro model ... 40
3.4 Hyaluronic acid influence on normal and osteoarthritic tissue-engineered cartilage ... 72
4 Summary and Outlook... 90
5 Kurzzusammenfassung ... 92
6 References ... 94
7 Appendix ...103
7.1 Publication and conference contributions ...103
7.2 Curriculum vitae ...105
Despite increasing effort in finding efficient treatments for osteoarthritis (OA), which is a major cause of morbidity and loss of joint function in the elderly population, many patients with OA still suffer from pain symptoms and disability. Up to now, no medical therapy has been shown to clearly halt or reverse OA progression, the related extracellular matrix (ECM) degradation, and the joint cavity inflammation followed by it. Hyaluronic acid (HA) is a main component of articular cartilage that endows synovial fluid (SF) with its viscoelastic properties and thereby provides lubrication for the articular surfaces. As OA progresses, inflammatory cytokines such as tumor necrosis factor-α (TNF-α) and interleukins are released, which lead to ECM degradation and reduction of specific cartilage matrix proteins such as collagen type II and aggrecan. At the same time, natural HA concentration decreases, which deteriorates the mechanical/viscoelastic properties of the SF. Intra-articular HA administration, the standard treatment of OA, aims to restore these properties, although HA is prone to enzymatic digestion and there is controversy over its underlying attributes. Slowly degradable injectable hydrogels with tunable mechanical and anti-inflammatory properties may pose a promising approach. Dendritic polyglycerol sulfate (dPGS), which has shown to prevent inflammatory responses, is used in this work to form a hydrogel through crosslinkage of dPGS-N3 with polyethylene glycol-dicyclooctyne (PEG-DIC) in a cytocompatible reaction. The viscoelastic properties of the obtained gels can be effectively tuned by varying the molar ratio of the building blocks. Since preserving and restoring the smooth articular surface is a primary goal of OA therapy, the tunable mechanical potential of dPGS-based hydrogel combined with its anti-inflammatory properties could be used to influence the OA alterations in a therapeutic sense. Therefore, the main topic of this study was to determine a suitable concentration for intra-articular injections of dPGS hydrogel that mimics HA in terms of its viscoelastic/mechanical properties, characterize the biological influence of the dPGS-based hydrogel on normal and OA-like tissue-engineered cartilage, and compare it with clinically used HA.
1.1 Synovial joint
Joints can be classified functionally or structurally, based on how much movement they allow and what kind of tissue structure is present in the joint, respectively. Structurally categorized, synovial joints are the most common type in the body, linking the musculoskeletal system and
facilitating its movement. The synovial joint consists of SF within a cavity surrounded by articular cartilage and synovial membrane (Figure 1).
1.1.1 Synovial membrane
Synovial membrane also called synovium is a vascularized, thin layer of connective tissue consisting of macrophage-like (type A) and fibroblast-like (type B) cells embedded in an ECM composed mainly of HA, collagen, and proteoglycans. The fibroblast-like cells provide the ECM that supports the structure of the synovium and are responsible for producing the viscous SF that lubricates the joint during movement and nourishes avascular cartilage. The tissue-specific function of macrophages is presumed to be included in joint homeostasis. Joint injury and disease affecting the blood-joint barrier may impair the process of SF formation, resulting in pathologic SF. Furthermore, in pathological situations, activated synovial cells are known to amplify the release of enzymes and factors that contribute to the destruction of the cartilage matrix.
1.1.2 Synovial fluid
A key structural characteristic for a synovial joint is the presence of a joint cavity that is not seen at fibrous or cartilaginous joints. This space is filled with SF (synovia = “a thick fluid”), a protein-rich fluid (a blood plasma dialysate), containing lubricant molecules, mainly hyaluronic acid (HA) and proteoglycan 4 (PRG4, also known as lubricin and superficial zone protein).
SF is secreted into the joint cavity by fibroblast-like cells of the synovial membrane,
and provides lubrication to reduce friction between the articular cartilage surfaces at bone ends. Furthermore, it facilitates the transport of nutrients and waste products including proteins and metabolites between the vascularized synovial membrane and the avascular cartilage.
1.1.3 Articular cartilage
The glassy, highly specialized connective tissue at the end of the bones in synovial joints is termed articular cartilage. Articular cartilage is avascular, aneural, and alymphatic with a low cell density, which contributes to limited intrinsic repair capacity. Therefore, even minor injuries may lead to progressive damage and joint degeneration that result in significant pain and disability.[16-17]
Structure and composition
Due to changes in structure and composition of articular cartilage, it has been divided into four distinct zones; (I) the superficial zone, (II) the transitional or middle zone, (III) the deep or radial zone, and (IV) the zone of calcified cartilage. These layers consist of water (up to 80% of wet weight in the surface zone and 65% within the deep zone), collagen (10-15% of wet weight,) and non-collagen proteins (5-10% of wet weight). The synthesis, maintenance, and degradation of these proteins are managed by chondrocytes, the only cell type in cartilage (5% of tissue volume). There are five collagen types present in the articular cartilage;
collagen II, VI, IX, X, and XI with type II being the most abundant one that makes up 95% of the solid composition of the mature human articular cartilage. The most abundant non- collagenous components in mammalian cartilage are proteoglycans (PGs). The basic PG unit consists of a core protein with one or more covalently attached glycosaminoglycan (GAG) chains including chondroitin sulfate, keratin sulfate, and HA. The most abundant PG in mature articular cartilage is aggrecan (Figure 1).
Figure 1.Schematic representation of the synovial joint and native articular cartilage. In articular cartilage, cells in the tangential zone are aligned parallel to the articular surface, cells in the middle zone are spherical and randomly distributed, while cells in the deep zone are aligned perpendicular to the tidemark and calcified zone and integrate with the subchondral bone. The matrix consists of a network of type II collagen fibers, which is reinforced by crosslinks formed between chains of hyaluronic acid, proteoglycans, and other non-collagenous proteins. Adapted from reference .
The dynamic functioning of synovial joint is facilitated by the presence of articular cartilage and is related to its mechanical and biomechanical properties. Type II collagen, the main structural protein of articular cartilage, arranges a meshwork that is sustained by non- collagenous proteins (such as cartilage oligomeric matrix protein) and other collagen types.
This network endows cartilage with tensile strength and provides a low-friction bearing surface that prevents bone-to-bone contact.[21-22] Water, absorbed by aggrecan and other embedded proteoglycans within this matrix, provides compressive resistance and permits a degree of shock absorbance during vigorous activities. Cartilage architecture and biochemical composition are arranged by chondrocytes. In undamaged conditions, chondrocytes are in a quiescent state holding a fine balance between synthetic and catabolic activities. However, degenerative joint diseases, traumatic cartilage injuries, and aging result in loss of homeostatic conditions and up-regulation of catabolic pathways.[23-24]
OA is the most common degenerative joint disease worldwide, which affects about 40 million people in Europe. Although OA can affect every synovial joint, it is more frequent in the knee, hip, spine, and hand. It is characterized by pain, transient morning stiffness (reduced mobility), and crepitus on joint motion (a cracking sound or sensation produced in the joint).
OA can be classified as primary (idiopathic) and secondary. Primary OA does not have any identifiable cause, such as an injury and results from a combination of risk factors with increasing age and obesity being the most prominent. Secondary OA is based on the attribution to recognized causative factors such as trauma and surgery on the joint structure. It is known that prior to the age of 40, the incidence is lower and mostly secondary OA occurs, commonly due to trauma. The prevalence increases between 40 and 60 years of age, and afterward a linear increase in the prevalence in later ages is observed. It is estimated that 9.6% of men and 18% of women of 60 or older probably have symptomatic OA.
Understanding the pathophysiology of OA is still evolving, from being considered as cartilage-limited to a multifactorial disorder that disturbs the whole joint, including alteration in the articular cartilage, subchondral bone, ligaments, capsule and synovial membrane, ultimately leading to joint failure. Cartilage degradation in OA can become stimulated as the result of a complex interplay of genetic, environmental, metabolic, and biochemical factors. However, the exact underlying mechanism is still unclear. Dysfunctional
chondrocytes and cartilage damage play a key role in the development of synovial inflammation. Proteinases released by chondrocytes lead to the formation of pro- inflammatory cartilage debris. These pieces of debris interact with other receptors on chondrocytes such as integrins and toll-like receptors and thereby enhance the expression of inflammatory and catabolic products. As they are in the synovial fluid, they act on the synovium to induce inflammation that in turn generates additional catabolic products. These products feedback on chondrocytes to further deregulate their function.
There are several main factors that drive OA progression including pro-inflammatory cytokines (IL-1β, TNF-α), chemokines, ECM degrading enzymes, such as matrix metalloproteinases (MMPs), which degrade collagen, and aggrecanases (a disintegrin and MMP with thrombospondin motifs (ADAMTS)). These enzymes are downstream key players in the inflammatory signaling cascade. Thus, the synovial cells, as well as the chondrocytes themselves, are potential sources of cytokines that could induce chondrocytes to synthesize and secrete cartilage-degrading proteases and other OA mediators. The biochemical changes together with biomechanical alterations disturb cartilage homeostasis and contribute to OA pathogenesis.
Another hallmark of degenerated cartilage is the phenotypic shift of chondrocytes toward hypertrophy. In addition, osseous outgrowths (osteophytes) often formed at the joint margins, subchondral bone sclerosis, meniscal tear and extrusion, and synovial membrane inflammation (synovitis) may also happen due to the mechanical changes during OA (Figure 2). Finally, all these implications lead to pain and loss of joint function.
Figure 2. OA cartilage. (a) The changes of articular structure during OA pathogenesis. (b) Cellular responses in OA-cartilage.
1.2.1 Main factors and players
The risk factors for OA can be divided into those that act at the level of personal awareness and those that change the biomechanical stability of the joint. Person-level risk factors include aging, female sex, genetic factors, joint biomechanics, and obesity. The main joint-level risk factors are joint injury, repetitive joint use through leisure or occupation, and joint malalignment. The Osteoarthritis Research Society International (OARSI), which is the premier organization in this field, has summarized three prevailing risk factors for OA in its 2017's summit. These include joint injury and altered biomechanics, aging, and systemic metabolic derangement (Figure 3). In this section, several important factors and their association to the compromised OA situation are introduced.
An important link between primary causes of OA is interleukin 6 (IL-6). Inhibition of IL-6 receptor with a monoclonal antibody, which is likely mediated by attenuated signal transducer and activator of transcription 3 (STAT3) signaling, reduce cartilage lesions and synovitis. IL-6 also increases the production of MMPs (-1, -3, -13) and aggrecanases (ADAMTS-4 and -5) in chondrocytes. IL-6 can induce and reciprocally be induced by basic calcium phosphate (BCP), which is found in the SF of almost 50% of OA patients.
Induction of IL-6 by BCP seems to form a positive feedback loop leading to cartilage damage, but the exact mechanism of how BCP crystals activate the chondrocytes remains unclear.
Recently, some studies suggested a role for mitochondrial dysfunction in OA pathogenesis. Kim et al. uncovered a regulatory network between mitochondria, lysosomes, and peroxisomes and found that this interconnectedness is potentially mediated by fission protein 1 (Fis1), which is reduced in human OA chondrocytes.
It is still a matter of debate whether metabolic derangement is a primary cause of OA.
Animal models showed that diet-induced obesity or hypercholesterolemia can lead to OA-like changes. Binding oxidized low-density lipoprotein (oxLDL) to the lectin-like oxidized- LDL receptor 1 (LOX-1) during inflammation and oxidative stress increases the production of reactive oxygen species in articular chondrocytes. Loss of LOX-1 is protective against OA- related damage.
Sirtuins (SIRTs) are deacetylases that play important roles in DNA repair. SIRT1 promotes chondrocyte survival and its loss corresponds to the disease stage. SiRNA- mediated knockdown or pharmacologic inhibition of SIRT1 leads to lower levels of transcripts for the clock gene Bmal-1, which controls cartilage homeostasis. This correlates with increased cartilage damage.
Rela/p65 is a key player in NF-kB signaling, which maintains chondrocyte homeostasis, with important roles in regulating the expression of SOX9 and ADAMTS5. Deletion of Rela results in acceleration of OA-related joint damage, which mostly is mediated by increased chondrocyte apoptosis.
Macrophages play an important role in the homeostasis of the healthy joint and mediate the pro-inflammatory and catabolic effects of alarmins (danger signals) by influencing factors such as TNF-α and IL-1β. The superficial zone (SZ) cells that express PRG4/lubricin may also be significant in tissue homeostasis and repair by migrating to the site of injury.
Fibulins are known to have functions in maintenance of basement membrane organization and elastic fiber formation. With age, fibulin 3 expression is decreased, which is associated with lower expression of PRG4. Fibulin 3 may be a trigger for lubricin maintenance and therefore important for maintaining progenitor cells in the SZ but can be lost with injury or aging.
Aging also leads to accumulation of senescent cells (SnCs) in the SZ. SnCs have a senescence-associated secretory phenotype (SASP), which includes the production of IL-6.
As OA develops, cartilage fibrillates and releases ECM fragments/debris into the joint.
Crystals that can be part of this debris induce and maintain an inflammatory cycle.
Interrupting these cycles by lubricants/viscosupplements may contribute to avoid OA progression.
Figure 3. Schematic summary of significantly associated primary causes (risk factors) for OA. Primary causes include injury and altered biomechanics, ageing, and systemic metabolic derangement (e.g., hypercholesterolemia). Green indicators represent a positive effect (protective against OA). Red indicators represent a negative effect (promoting OA). Arrows indicate a positive relationship (stimulatory effect), whereas blunt-ended arrows indicate an inhibitory effect. Based on reported evidence from the 2016-2017 literature.
1.2.2 Conventional treatments
There is no cure for OA available up to now and the desired therapeutic goal is to fight against clinical symptoms and, if possible, to inhibit the progression. Different interventions are available for OA management, including non-pharmacological (lifestyle changes), pharmacological and surgical methods. Patients who cannot gain sufficient pain relief and do not retrieve joint function by non-operative methods should be considered for the ultimate OA treatment: the prosthetic replacement of the affected joint. The first line of treatment considered by American College of Rheumatology (ACR), European League Against Rheumatism (EULAR) and OARSI guidelines are currently the non-pharmacological therapies. The most widely proposed in this category are listed in Table 1.
Table 1. Most widely proposed non-pharmacological therapies for osteoarthritis.
Aerobics Weight reduction Thermal modalities
Walking aids Muscle strengthening Acupuncture
Transcutaneous electrical nerve stimulation
Education and self- management
Referral to a physical therapist
Non-pharmacological therapies are not sufficient to achieve sustained pain relief and restoration of the joint function in many OA patients, which led to development of various pharmacological treatments including both the fast and slow-acting drug families (Table 2).
Table 2. Most widely proposed pharmacological therapies for osteoarthritis.
Fast-acting drugs Slow-acting drugs
Acetaminophen (paracetamol) Glucosamine
Non-steroidal anti-inflammatory drugs (NSAIDs) Chondroitin sulfate Cyclooxygenase-2 (Cox-2) inhibitors S-adenosylmethionine
Glucocorticoids Avocado/soybean unsaponifiables
Opioids Hyaluronic acid
The fast-acting drug family is mainly used for pain relief and to alleviate inflammation.
The first stage of treatment consists of analgesics such as acetaminophen, however, it can trigger adverse hepatic events in patients with hepatic insufficiency. Non-steroidal anti- inflammatory drugs (NSAIDs) and cyclooxygenase inhibitors (also called coxibs) are typical anti-inflammatory compounds that are used as analgesic treatments. However, NSAID are associated with gastrointestinal (nausea, vomiting, and constipation), renal and cardiovascular toxicity. Intra-articular administration of glucocorticoids can rapidly eliminate joint effusion after inflammation, but is associated with a high risk of infection and exhibits adverse metabolic events. Opioids are only used if other drugs do not provide sufficient pain relief and for patients with intolerance to other pharmacological treatments. However, they show a wide range of adverse events such as gastrointestinal dysfunction, alteration in the cognitive function, dependence, and respiratory depression. In addition, there is the group of slow-acting drugs in osteoarthritis (SADOA) with long lasting effects, such as pain prevention as well as attenuation of cartilage destruction (e.g., HA, glucosamine, chondroitin sulfate). The effects of SADOA are not yet clear but are known to have several anti- inflammatory properties that block the pain receptors and may have influence on the viscoelastic properties of the cartilaginous tissue. The use of viscosupplementation is growing worldwide due to the positive effects on pain relief, lubrication, and joint functional amelioration.
1.2.3 Viscosupplementation with hyaluronic acid
HA is a major component of the SF, which acts as a shock absorber to protect the cartilage against mechanical injuries. It endows SF with its viscoelastic properties and thereby provides lubrication for the articulating surfaces. HA is an anionic, nonsulfated glycosaminoglycan,
composed of repeating D-glucuronic acid and N-acetyl-D-glucosamine. It can bind to large amounts of water and it is found in human synovial fluid in a macropolymeric form with an average molecular weight of 3–4 million Dalton. As OA progresses, natural HA concentration decreases into the lower ranges of HA molecular weight, leading to a deterioration of the mechanical/viscoelastic properties of the SF. Viscosupplementation with HA, the standard treatment for OA, aims to restore these properties. The pain relief may be due to the improvement of viscoelastic or mechanical properties of SF, i.e., lubrication, resistance to shear, and cushioning for the joint. Others propose biological mechanisms of action beside shock absorption and joint lubrication, including, anti- inflammatory effects, chondroprotection, proteoglycan synthesis, and cartilage matrix alterations. Understanding these HA-related modifications on cellular and molecular level may serve as a guide for the development of future therapies. Regardless of its mechanism of action, this natural polymer is prone to uncontrolled enzymatic degradation. There are currently two types of HA available on the market, namely; low molecular weight (LMW) HA (0.5–3.6 million Da) and chemically crosslinked high molecular weight (HMW) HA (6.0 million Da) hydrogels. It has been reported that non-modified LMW HA has a half-life of only 10–13 h in osteoarthritic patients, while chemically modified HA hydrogels, such as hylan G-F 20, and genzyme can last for around 9 days. The future viscosupplementation approaches need to have sufficient long-term action at the injection site for sustained efficacy.
Moreover, several injections should be avoided to minimize infection risks and costs. For optimal treatment of an OA joint, the local environment of the entire joint needs to be reset to the physiological baseline.[63, 66] To this end, an injectable hydrogel approach that addresses the joint resurfacing, inflammation, and mechanical issues may offer a successful approach.
Hydrogels are 3D crosslinked polymer systems capable of absorbing large amounts of water to form aqueous semi-solid gel networks. They can be tuned with regard to their chemical nature, physical structure, sensitiveness to external stimuli, and biocompatibility. They can be classified into different groups based on their:
⇒ crosslinks: physically or chemically crosslinked
⇒ electric charge: ionic (charged) or neutral
⇒ fate in the organism: degradable and slow-degradable
⇒ origin: synthetic, natural, or hybrid
⇒ responses to external effects: stimulus-sensitive and -responsive
The term hydrogel as we know it today was first introduced by Wichterle and Lim in 1960 for use as soft contact lenses. Over the past decades, significant improvement has been made in designing and application of hydrogels as functional biomaterials including pharmaceutical, biomedical, and drug delivery systems. The consistency (building blocks and concentration of physical or covalent crosslinking), degradability, and biochemical properties are important design criteria that can influence the structural, mechanical, and biological properties of the hydrogels initially and over time. In addition, the hydrogel building blocks must be stable in either solid or solution form for storage prior to use.
Hydrogels are considered to be biocompatible in general due to their high water content, and low interfacial tension with the surrounding biological environment. In some cases they even mimic the native ECM both compositionally and mechanically. The swelling ratio, which has a major impact on the biological environment, depends on several factors like the osmotic pressure inside the hydrogel and the crosslinking density. For example, osmotic pressure can be changed with the deprotonation of carboxylic acids due to a pH change, whereas crosslinking density changes with the network degradation.
A growing field for injectable hydrogels is the application in treatment of cartilage- related diseases. Since they fit into any desired form, injectable hydrogels can match the usually observed irregular cartilage defects. This way, they might replace implantation surgeries in cartilage by minimal invasive injections. A variety of chemical or physical crosslinking strategies can be used to form injectable hydrogels, but they must be carefully selected to match the specific application. For example, a suitable crosslinking rate is necessary for the proper formation of an injectable hydrogel in situ. If the gelation is too fast, premature gel formation in the syringe may occur, resulting in network defects that affect gel mechanical properties and can clog the syringe. On the other hand, if the gelation is too slow, precursors are likely to perfuse from the injection site into surrounding tissues, causing poor hydrogel properties and potentially an inflammatory response to unreacted monomers.
Furthermore, the ability to form the hydrogel in the presence of living cells without interfering with native biochemical processes (bioorthogonal chemistry) is a key feature for cell biomedical applications. Different approaches are available for the fabrication of such injectable hydrogels. Among them, click chemistry is the most researched chemoselective crosslinking reaction (refer to 'Hydrogel formation by click chemistry' in section 1.3.1).[29, 78]
1.3.1 Injectable hydrogels for viscosupplementation in osteoarthritis
The choice of material and appropriate fabrication method play crucial roles in developing ideal injectable hydrogels that can function as viscosupplement (lubricant) in OA. A variety of materials, both natural and synthetic, have been exploited to prepare injectable hydrogels for this purpose, leading to two main hydrogel categories; HA-based and non-HA-based hydrogels (Table 3).
Injectable HA-based hydrogels for viscosupplementation in osteoarthritis
To overcome the poor mechanical properties, fast degradation, and hydrolytic reactions of HA, this natural polymer is usually modified or combined with other materials. In one approach, the HA backbone is derivatized with hexadecylic side chains, through amide bonds, with a 1–3 mol-% degree of substitution of repeating units, resulting in a stable hydrogel.
HYADD4® forms a gel at a concentration of 0.3% (w/v) in PBS, using no chemical crosslinking. Therefore, the biocompatibility and safety issues related to crosslinking techniques are eliminated. Hymovis® (8 mg/mL aqueous formulation of HYADD4®) has proven to be effective in reducing the signs and symptoms of pathology and in protecting cartilage in animal studies. Recently Hymovis® has shown to be effective and safe for patients as well. Furthermore, HA-based hydrogels can be designed for dual purposes;
viscosupplementation and intra-articular drug delivery into joints (localize the curative constituent). For example, recently Xia et al. showed that HA methacrylate can be photo- crosslinked with chitosan microspheres encapsulating cordycepin (an inhibitor of ADAMTS- 5 and MMP13). This hydrogel ameliorated the progression of surgically-induced OA. A crosslinked HA hydrogel in combination with dexamethasone reduces the toxicity of this drug. In another study, a hyaluronat, chondroitin sulfate, N-acetyl-D-glucosamine compound in hydrogel form has shown more chondroprotective effects to rats' cartilage when compared to HA during the early stages of OA. HA polymer grafted with antioxidant molecules led to a decrease in synovial membrane hypertrophy. More examples can be found in Table 3.
Injectable non-HA-based hydrogels for viscosupplementation in osteoarthritis
Based on the knowledge of HA and HA-based hydrogel, researchers began to investigate other hydrogels with chemical and physical constructions resembling HA to extend the viscosupplementation effects. Recently in 2017, Milcovich and colleagues reduced the on-site enzyme degradation by optimizing a polysaccharide-based colloidal hydrogel. In this study,
zwitterionic vesicles were proposed as a physical crosslinker that caused the formation of a tunable network, offering a dual-therapeutic approach. More examples can be found in Table 3.
Table 3. HA-based and non-HA-based hydrogel approaches for viscosupplementation in OA.
Main components Advantages Ref.
Crosslinked HA Providing drug delivery matrix for conjugate drugs
Hexadecylic side chain derivative of HA
Omission of chemical crosslinking drawbacks
HA + cordycepin (inhibitor of ADAMTS-5 and MMP13).
Inhibition of OA progression 
Hyaluronat, chondritin sulfate, N-acetyl-D- glucosamine
Chondroprotective effect 
HA+ dexamethasone Reduction of drug toxicity 
HA + antioxidant molecules Reduction of the synovial membrane hypertrophy
HA + corticosteroid Rapid and long lasting pain relief
HA + doxycycline Long-lasting drug agent Restoring the elastoviscosity
Thioethyl ether derivative of HA
Radical protective 
HA + chitosan Prevention of subchondral bone loss
Poly caprolactone + chitosan + Etoricoxib (COX-2
Reduction of drug toxicity Longer retention time
Alginate + chitosan Reduction of the synovial membrane inflammation Prevention of OA development
Polysaccharide-based colloidal hydrogel
Reduction of on-site enzyme degradation
Hydrogel formation by click chemistry
Click chemistry is a term that was introduced by Sharpless et al. in 2001 to describe pairs of functional groups that rapidly and selectively react (click) with each other that give high yields without side-products and generally require no purification. Due to its rapid crosslinking kinetics, high efficiency, unique bioorthogonality, and mild reaction conditions, click chemistry represents one of the most attractive classes of crosslinking chemistries for the formation of hydrogels with varying dimensions and patterns (Figure 4).
Figure 4. Preparation and potential biomedical applications of click hydrogels, microgels and nanogels.
Among the different click reactions, the copper-catalyzed alkyne–azide reaction (CuAAC) is the most investigated method, which is a [3+2] copper-catalyzed cycloaddition reaction between an azide and an alkyne to form a 5-membered triazole ring. However, copper can be toxic, which limits its application in the biomedical field.
To overcome this, Bertozzi et al. crosslinked cyclooctynes and azides by copper-free click chemistry using strain-promoted azide-alkyne cycloaddition (SPAAC) reactions, thereby eliminating the need of (metal ion) catalysts. DeForest and Anseth showed that when a four-arm PEG is end-functionalized with difluorinated cyclooctyne, it can react with an azide- functionalized crosslinker, via SPAAC. The ring strain and electron-withdrawing fluorine
substituents promote a rapid crosslinking reaction (~2 minutes) without a catalyst. They were able to prove that the timescale and mechanism of the SPAAC reaction permits high viability (>95%) during encapsulation of both cell lines and primary cells. In another approach, Ito et al. reported the preparation of covalently crosslinked, degradable HA hydrogels using azide and cyclooctyne functionalized precursors (Figure 5).
Figure 5. In situ copper-free click reaction using strain-promoted hyaluronic acid precursors.
1.3.2 Polyethylene glycol and dendritic polyglycerol sulfate as building blocks for injectable in situ hydrogels
Biocompatible natural polymers like HA mimic aspects of the native microenvironment, including its mechanical and biochemical properties for regulating cell adhesion, migration, and other key functions for tissue repair. Nevertheless natural polymers possess batch-to- batch variations, moderate yield through tedious processes, and inferior mechanical properties. Furthermore, they are prone to uncontrolled enzymatic degradation. To address these shortcomings, synthetic polymers have been frequently used for the design of injectable, cell-compatible hydrogels due to their commercial availability, low batch-to-batch variation, versatility for chemical modification, and therefore, the ease of tuning the mechanical properties of the resulting hydrogels.
Polyethylene glycol (PEG)
PEG, a biocompatible polymer with a variety of biomedical applications, is able to protect encapsulated cells from the host's immune response.. PEG-based hydrogels have been successfully studied for the encapsulation of a broad range of cell types, including chondrocytes. End hydroxyl functional groups of PEG could be substituted by other groups to obtain polymers for different applications. Accordingly, cyclooctyne could be attached to the end groups of PEG to obtain PEG-DIC. This derivative of PEG is highly reactive and therefore a useful reagent for biocompatible copper free reactions, where no active oxygen is generated as a result of copper salt addition.
Dendritic polyglycerol sulfate (dPGS)
Dendrimers are highly branched, monodisperse macromolecules with well-defined structures which affect their physical and chemical properties. Dendritic polyglycerol (dPG) is a hydrophilic, low-toxic branched polymer containing multiple hydroxyl (OH) groups on the periphery. The hydroxyl groups can be easily functionalized and changed to other functional groups. This surface multifunctionality offers the opportunity for multivalent interactions with biological substrates and thereby makes them valuable crosslinkers for preparation of multifunctional polymeric hydrogels. In 2004, the Haag group developed a heparin mimetic sulfated branched polymer (dPGS) in one step by sulfation of dPG. This dendritic fully synthetic analogue of heparin/heparan sulfate proteoglycans is a promising candidate to mimic ECM. The main advantages of dPGS over the other heparin mimetic scaffolds are high functionality, a gram scale and straightforward synthesis, as well as control over the degree of sulfation, which leads to an anti-inflammatory property and low anticoagulant activity. dPGS showed inhibition of the complement system (C3a and C5a), L-and P-selectin inhibition, and inflammation targeting in an arthritis model.
Previously, Schulze-Tanzil and colleagues have demonstrated a chondroprotective and anti- inflammatory potential of dPGS nanoparticles in the osteoarthritic knee joint suitable to suppress OA progression. Following these results, it would be very interesting to use a dPGS-based hydrogel instead of nanoparticles for more resilience.
It is possible to crosslink dPGS-N3 units with PEG-DIC by a SPAAC reaction to form an injectable hydrogel (Figure 6).
Figure 6. PEG-DIC and dPGS-N3 can be used as hydrogel blocks for in situ crosslinking by SPAAC to construct dPGS hydrogels.
This reaction does not need any external stimuli/triggers for the initiation and has proven to be cytocompatible in a previous study, in which human chondrocytes were encapsulated in dPGS-based hydrogels over 21 days. The anti-inflammatory biological signals provided by sulfate groups to diminish an inflammatory processes can initiate the reparative processes and prompt the patient’s own tissue to complete its regeneration. The viscoelastic properties of such a hydrogel can be effectively tuned for a certain purpose by varying the molar ratio of the building blocks. Furthermore, this gelation procedure allows the in situ formation of hydrogels from injectable solutions. Unlike natural polymers, this fully synthetic hydrogel possesses superior mechanical properties and is not prone to uncontrolled enzymatic degradation since slowly-degradable linkers can be used in this approach. All these features make dPGS-PEG hydrogel superior to natural analogue and a good alternative for future approaches in OA viscosupplementation.
1.4 In vitro investigation of potential treatments for OA
Disease models are fundamental to advance research about the underlying causes of the disease, and for testing of potential therapeutics. Both in vivo and in vitro models for OA have been used in the past. In vivo models provide the most authentic reflection of the
whole-joint disease, but they are time consuming, expensive, and difficult to control. In contrast, in vitro models can be applied to examine novel therapeutic strategies in cartilage repair offering a cost effective analysis of potential substances in high throughput approaches under standardized conditions. They attempt to mimic factors and conditions, which trigger OA or analyze the underlying pathways. Additionally, they offer the opportunity to study early features of the OA development that have been difficult to investigate due to the lack of available tissue from early disease and restricted molecular changes associated with it.
The ease of manipulating such systems, as well as a shift towards the 3R philosophy of refining, reducing, and replacing the use of animals, make in vitro models attractive. Even though a great variety of in vitro models have been used by researchers, no consensus has emerged on the most appropriate model yet. The relevance of in vitro models to actual disease needs to be carefully interpreted. For instance, some publications show the chondroprotective effects of glucosamine and chondroitin sulfate in in vitro models,
whereas clinical trials do not show such effects in vivo. Although some of these differences can be attributed to delivery, complexity, duration, and variation of the phenotype, the in vitro models should be improved to better reflect the natural disease in vivo.
In vitro models can be categorized based on the trigger among which cytokine stimulation (cytokine-based) and load-based models are the most prevalent. The signaling pathways induced by cytokine- and load-based induction are similar in both models.
1.4.1 Load-based in vitro models
Chondrocytes sense the loading of their environment through integrin receptors, which lead to cytoskeletal disruption and release of cytokines. These cytokines then cause a release of enzymes, which cleave the ECM proteins. The degraded proteins are then capable of further induction of matrix degradation. Static loading can induce changes and create an OA model when applied at an appropriate magnitude. Therefore, identification of the load thresholds that alter the balance from maintenance of homeostasis to catabolic degradation is important. For instance, static compression of calf cartilage to 25% or 50% strain for 24 h produces destructive alterations in cartilage metabolism, resulting in an over expression of MMP3, -9, and -13 and a decrease in COL2A1 and ACAN. However, in such models, either the cytokine or the cytokine-producing cells should be added, otherwise the model cannot replicate inflammatory processes. Load-based models need extra operational equipment and set ups, which leads to limited applicability. Moreover, due to this limitation, the magnitude of experiments and thereby high-throughput readouts are usually impeded.
1.4.2 Cytokine-based in vitro models
During OA, the increase in catabolic proteins is followed by stimuli such as cytokine or chemokine exposure, including IL-1β and TNF-α, which are present in the diseased joint.
Such cytokines represent ideal candidates for the induction of OA-like biological changes.
Cytokine-based models are commonly used and generally well understood. The model is usually inexpensive and easy to manipulate. Cell expansion in vitro allows for a magnitude of experiments and therefore, testing multiple hypotheses and parameters from single sources of tissue is possible. Nevertheless, primary chondrocytes undergo dedifferentiation after only a small number of passages during which they lose their phenotype and their ability to form ECM. IL-1β and TNF-α are the most commonly used cytokines in OA in vitro models. Other cytokines such as IL-6, IL-8, and VEGF play a role as well and are increased in the synovial fluid of OA joints. However, they are hardly ever considered in model design because their production can be induced by other cytokines, such as IL-1β or TNF-α.
The most commonly used in vitro models include ex vivo tissue culture (explants), monolayer culture, 3D culture, and co-culture. The advantages and disadvantages of some of these models are listed in Table 4.
Table 4. Advantages and disadvantages of some of the most commonly used in vitro models.
Model type Advantages Disadvantages Ref.
Allows expansion from a single sample, investigation of distinct pathways in isolation
Altered phenotype of isolated cells due to isolation from tissue and absence of normal ECM
Co-culture Considers cross-talk between cell types
Altered phenotype of isolated cells Different cell types require different culture conditions, or a compromise if cultured together.
3D-culture Offers structure and force to sensitive cells
Magnitude of force is scaffold
dependent and may not reflect that of the normal tissue.
Isolation and expansion of cell types are still required.
Explant Inexpensive, easily produced, cells maintained in normal ECM
Cell death at cut edge of tissue, few replicates available from same source, more than one tissue type may be required to maintain viability, and physical attributes may change in culture.
In 2014, Schlichting et al. have introduced a scaffold-free in vitro OA model by using cells from porcine cartilage sources. They have thus developed an easy to manage OA model that mimics essential aspects of human chondrocytes and native cartilage biology, pathophysiology, and differentiation. In this model, 3D chondrocyte micromasses are cultured for 14 days to form ECM and then stimulated for further 7 days with TNF-α to introduce OA- like changes, as well as the test substance (Figure 4). TNF-α addition established a degradative environment in line with the generation of macroscopic changes such as extensive proteoglycan loss as an implicit feature of human OA. Furthermore, gene expression profiling of porcine tissue-engineered cartilage micromasses revealed a human-like OA reaction pattern such as an extensive ECM loss (collagen type 2 (COL2A1), cartilage oligomeric matrix compound (COMP), aggrecan (ACAN)), cell death, formation of an inflammatory environment through the induction of genes coding for chemokines (IL-8, C-C motif chemokine 2 (CCL2)), OA-relevant enzymes (MMP1, -13), and the modulation of genes involved in skeletal development. These typical OA changes can be examined and documented by conventional methods. Microscopically, OA cartilage is characterized by loss of collagen and proteoglycans and these characteristics are analyzed in this model by collagen type II immune-staining and Safranin O staining, respectively. Further variations can be documented on gene expression level (Affymetrix porcine microarray and/or real time- polymer chain reaction (RT-PCR)), combined with a cell viability assay (Figure 7).
Figure 7. Schematic presentation of in vitro OA model.
2 Scientific goal
Injectable hydrogels are a promising approach to treat cartilage damage induced by OA, which has been remained a major orthopedic challenge. The viscoelastic properties of such hydrogels can be effectively tuned for a certain purpose due to the molar ratio of the building blocks. The aim of this study is to investigate the potential of a slowly degradable dPGS- based hydrogel as an alternative viscosupplement for OA management. Therefore, a characterization of the dPGS hydrogels that were newly developed in the Haag group should be carried out first. This includes, biological characterization, rheology measurements to determine a suitable concentration for intra-articular injections that mimics HA and a standard viscosupplement for OA, in terms of viscoelastic and mechanical properties. It also entails the potential underlying molecular and cellular changes and interactions with biological systems along with the hydrogel efficacy to alter the OA condition needs to be evaluated. This is possible by using in vitro OA-modeling, in regards to the parameters of cell viability, GAG content, collagen type II presence, and global gene expression profiling. Additionally, we compared the dPGS hydrogel with HA. The present conflicting data regarding the controversial effects of HA encouraged us to investigate more thoroughly the physiologic effect of HA on the cellular and molecular level, using the same unique in vitro model.
Furthermore, understanding these HA-related modifications may create a better understanding of how intra-articular HA treatment could lead to therapeutic effects.
Figure 8. Overview of the main objectives of this PhD thesis.
concentration for injection Physiological effects of HA
Hydrogel efficacy to alter OA-like condition
3 Publication and Manuscripts
In the following section the published articles are listed and the contributions of the authors are specified.
3.1 Hydrolytically degradable, dendritic polyglycerol sulfate based injectable hydrogels using strain promoted azide–alkyne cycloaddition reaction
Pradip Dey, Shabnam Hemmati-Sadeghi, and Rainer Haag, Polymer Chemistry 2016, 7, 375-383.
Figure 9. Covalent network formation by strain promoted azide–alkyne cycloaddition reactions. Adapted from reference .
In this publication, the author contributed to the acquisition, analysis, and interpretation of the biological data, and composed the related section in the manuscript.
3.2 Injectable hydrogels for treatment of osteoarthritis – A rheological study
Benjamin von Lospichl,# Shabnam Hemmati-Sadeghi,# Pradip Dey, Tilo Dehne, Rainer Haag, Michael Sittinger, Jochen Ringe, Michael Gradzielski, Colloids and Surfaces B:
Biointerfaces 2017, 159, 477-483.
# Authors contributed equally.
The rheological properties of a slowy degradable dPGS hydrogel have been investigated to determine a suitable concentration for intra-articular injections. The oscillating and flow rheology showed an overall polymer concentration of 4.0 wt% dPGS hydrogels have similar viscoelastic properties to HA, the current standard viscosupplement for OA management.
Figure 10. Rheology comparison between dPGS hydrogel and HA.
In this publication the author contributed to the concept, sample preparation, and rheology measurements, and composed parts of the manuscript.
3.3 TNF-induced biomimetic sulfated PEG-hydrogel inhibits proteoglycan loss and TNF-induced expression pattern in an osteoarthritis in vitro model
Shabnam Hemmati-Sadeghi, Pradip Dey, Jochen Ringe, Rainer Haag, Michael Sittinger, and Tilo Dehne, Journal of biomedical materials research part B-applied biomaterials 2018.
Figure 11. Viability and cartilage qualities.
In this publication the author contributed to the concept and experimental design, was responsible for acquisition, analysis and interpretation of the data, and composed the manuscript.
Biomimetic sulfated PEG hydrogel inhibits proteoglycan loss and TNF- induced expression pattern in an osteoarthritis in vitro model
Shabnam Hemmati-Sadeghi a,b, Pradip Dey b,d, Jochen Ringe c, Rainer Haag b, Michael Sittinger c,*, and Tilo Dehne c
a) Charité - Universitätsmedizin Berlin, corporate member of Freie Universität Berlin, Humboldt-Universität zu Berlin, and Berlin Institute of Health, Berlin-Brandenburg School for Regenerative Therapies
b) Institut für Chemie und Biochemie, Takusstraße 3, Freie Universität Berlin, 14195 Berlin, Germany.
c) Charité Universitätsmedizin Berlin, Tissue Engineering Laboratory & Berlin- Brandenburg Center for Regenerative Therapies, Department of Rheumatology, Charitéplatz 1, 10117 Berlin, Germany.
d) Polymer Science Unit, Indian Association for the Cultivation of Science, Kolkata, 2A and 2B Raja. S.C. Mullick Road, Kolkata - 700032, India
Name and contact details of the corresponding author:
Surname, First Name Sittinger, Michael Tel +49 30 450 513 198 Fax +49 30 450 513 957
Academic Address I. Charité Universitätsmedizin Berlin, Tissue
Engineering Laboratory & Berlin-Brandenburg Center for Regenerative Therapies, Department of
Rheumatology, Charitéplatz 1, 10117 Berlin, Germany
This study aimed to evaluate the potential of an anti-inflammatory PEG hydrogel for osteoarthritis (OA) management in an OA in vitro model.
Freshly isolated porcine chondrocytes were maintained high-density cultures to form cartilage-like 3D micromasses. Recombinant porcine tumor necrosis factor alpha (TNF- α) was used to induce OA-like changes. Normal and OA-like micromasses were treated with dendritic polyglycerol sulfate-based PEG hydrogel. Live/dead staining showed that all micromasses remained vital and presented similar morphological characteristics.
Safranin-O staining demonstrated a typical depletion of glycosaminoglycans in TNF- treated micromassbut not in the presence of the hydrogel. There was no distinct difference in immunohistochemical detection of type II collagen. Microarray data showed that rheumatoid arthritis and TNF signaling pathways were down regulated in hydrogel-treated OA-like micromasses compared to non-treated OA-like micromasses.
The hydrogel alone did not affect genes related to OA such as ANPEP, COMP, CXCL12, PTGS2, and TNFSF10, but it prevented their regulation caused by TNF-α. This study provides valuable insights toward a fully synthetic hydrogel for the intra-articular treatment of OA. The findings proved the potential of this hydrogel to prevent the development of TNF-induced OA with regard to proteoglycan loss and TNF-α-induced expression pattern without additional signs of differentiation and inflammation.
Keywords: microarray, hydrogel, dendritic polyglycerol sulfate, polyethylene glycol, tumor necrosis factor
Running Headline: dPGS hydrogel inhibits proteoglycan loss
To date, no cure is available for Osteoarthritis (OA).1 In the end-stage, treatment options are restricted to total joint replacements. In early stages, symptom management is possible with nonsteroidal anti-inflammatory drugs (NSAIDs) or hyaluronic acid (HA) to relieve the pain, facilitate movement and slow OA progression.2 Due to the positive effects of intra- articular injections of HA (viscosupplementation) on pain relief, lubrication, and joint functional amelioration, their use is growing worldwide.3 HA exhibits unique viscoelastic properties with highly non-Newtonian characteristics that provide the synovial fluid with the friction-reducing fluid dynamic properties (lubrication), as well as resistance to compression and shear forces.4,5 Unfortunately it is prone to uncontrolled enzymatic degradation6 that substantially restricts the sufficient long-term action at the side of injection.
Synthetically derived hydrogels offer a highly tunable platform to create biomimetic environments that support repair of damaged or diseased cartilage7 or to deliver drugs.8 Among them, dendritic polyglycerol sulfate (dPGS), which is a branded fully synthetic analog of heparin/heparan sulfate proteoglycans, is a promising candidate due to its high biocompatibility and presence of multiple sulfate groups on the periphery that act as an anti-inflammatory compound. dPGS has shown inhibition of complement system (C3a and C5a),9 L-and P-selectin inhibition,10 and inflammation targeting in an arthritis model.11 It is possible to cross-link dPGS azide (dPGS-N3) with polyethylene glycol-dicyclooctyne (PEG- DIC) to form an injectable hydrogel by a bioorthogonal strain-promoted azide–alkyne cycloaddition (SPAAC)12 reaction, that can be tuned with respect to its rheological properties. It has been shown that the dPGS-PEG hydrogel with an overall polymer
concentration of 4.0 wt% has the same viscoelastic properties as HA in the knee frequency range.5 Polyethlene glycol (PEG) is a biocompatible polymer that protects regenerative living cells from host immune response.13 PEG has been successfully studied for encapsulation of chondrocytes.14 All these features make dPGS-PEG hydrogel a good candidate for cartilage repair. In the present study, we investigated the potential of the dPGS-based hydrogel to alter the OA condition. In order to test the efficacy of our fully synthetic hydrogel, we used the porcine chondrocyte micromass culture model, which has been shown to be an alternative tissue platform for the evaluation of innovative substances and techniques for the treatment of OA.15 In this model, established normal micromass cultures were treated with dPGS-PEG hydrogel for 7 days under normal and OA conditions (by adding TNF-α.) Parameters such as cell survival, extra cellular matrix (ECM) formation or loss and changes in gene expression profiles were used to investigate the effect and to evaluate the potential to inhibit or alter the OA condition.15
Materials and Method
dPGS hydrogel formation: Basic components SO3pyridine complex and polyethylene glycol hydroxyl (PEG-OH) were used as received from company Fluka Production GmbH and Sigma Aldrich (Mn=6 kDa). PEG was further modified to homobifunctional polyethylene glycol-dicyclooctyne (PEG-DIC) and dendritic polyglycerol sulfate azide (dPGS-N3) at the Institute of Chemistry and Biochemistry of the Freie Universitaet of Berlin.
These two macromonomeric components are capable of in situ crosslinking by strain- promoted azide–alkyne cycloaddition (SPAAC) to construct dPGS hydrogels under physiological conditions, as shown in Figure 1.14,16 The components were prepared as solutions (2.5 wt%) in RPMI 1640 medium, and filtered through 0.2 µ filters (Sartorius) and
supplemented with 10% fetal bovine serum (FBS Thermoscientific, v/v), 100 U/mL penicillin and 100 µg/mL streptomycin (Biochrom) and 170 µM L-ascorbic acid (Sigma- Aldrich). The components were mixed in a 1:1 ratio and incubated at 37 °C for 60 min to form the hydrogel in situ.
Fig 1: Schematic presentation of the polymer structure involved in the hydrogel formation. Polyethylene glycol- dicyclooctyne (PEG-DIC) and dendritic polyglycerol sulfate azide (dPGS-N3) were used as macromonomers for in situ crosslinking by strain-promoted azide–alkyne cycloaddition (SPAAC) to construct dPGS hydrogels
Chondrocyte isolation and preparation of 3D micromasses: Since the samples were obtained from a slaughterhouse, no animal approval was needed. Chondrocytes were isolated from medial and lateral femoral condyle cartilage of domestic pigs (9 donors) according to a previously published protocol.17 Briefly, cartilage slices were incubated for 19 h in spinner flasks containing RPMI 1640 medium, supplemented with 10% fetal bovine
serum (FBS, Thermoscientific, v/v), 100 U/mL penicillin and 100 µg/mL streptomycin, 333.3 U/mL collagenase II (all Biochrom), 1 U/mL collagenase P (Roche Diagnostics), and 33.3 U/mL hyaluronidase (Sigma-Aldrich). Afterwards, incubated cell suspensions were strained through a nylon mesh with a 100 µm pore size (Becton Dickinson), washed in Hanks solution (Biochrom), and resuspended in a maintenance medium consisting of RPMI 1640, 10% FBS, penicillin/streptomycin, and supplemented with 170 µM L-ascorbic acid (Sigma-Aldrich). Before preparing micromasses, cells from three donors were pooled together and three independent pools were created serving as biological replicates (n = 3).
The high-density micromass culture (micromass), was described previously.15 Briefly, a volume of 200 µL containing 6*105 freshly isolated chondrocytes in maintenance medium was transferred to each well of 96-well flat bottom plates (Becton Dickinson). Micromasses were allowed to establish ECM for 14 days in all experimental groups and then were cultured for further 7 days under different conditions resulting in 4 experimental groups as following: (1) without stimulation (Ctr), (2) stimulated with 10 ng/mL TNF-α (R&D system) to induce OA-like changes (TNF), (3) treated with 2.5 wt% hydrogel in medium (Gel), and (4) treated with 2.5 wt% hydrogel in medium and 10 ng/mL TNF-α (GelTNF).
Live/dead staining: Propidium iodide/fluorescein diacetate (PI/FDA) staining (Sigma) was performed to evaluate the cell viability of the micromasses. The micromasses were rinsed with phosphate buffered saline (PBS, Biochrom) and incubated for 15 min at 37 °C with 3 µg/mL FDA solution. After incubation, the micromasses were rinsed again with PBS and incubated with 100 µg/mL PI solution for 2 min at room temperature and under darkness. After an additional washing step, the micromasses were analyzed under a fluorescence microscope (Olympus AX70). As a result, living cells were green and the nuclei